www.ijmer.com

International Journal of Modern Engineering Research (IJMER) Vol.3, Issue.3, May-June. 2013 pp-1330-1335 ISSN: 2249-6645

Optimisation of Weld Bead Parameters of Nickel Based Overlay Deposited By Plasma Transferred Arc Surfacing Er. Bhaskarananda Dasgupta, 1 Dr. Sudip Mukherjee2 1

Assistant Professor, Department Of Mechanical Engineering Siliguri Instiotute of Technology, Siliguri, West Bengal India Professor, Department Of Mechanical Engineering, Jalpaiguri Government Engineering College, Jalpaiguri, West Bengal, India

2

Abstract: Plasma Transferred Arc surfacing is a kind of Plasma Transferred Arc Welding process..Plasma Transferred Arc surfacing (PTA) is increasingly used in applications where enhancement of wear, corrosion and heat resistance of materials surface is required. The shape of weld bead geometry affected by the PTA Welding process parameters is an indication of the quality of the weld. In this paper the analysis and optimization of weld bead parameters, during deposition of a Nickel based alloy Colmonoy on stainless steel plate by plasma transferred arc surfacing, are made and values of process parameters to produce optimal weld bead geometry are estimated. The experiments are conducted based on a five input process parameters and mathematical models are developed using multiple regression technique. The direct effects of input process parameters on weld bead geometry are discussed using graphs. Finally, optimization of the weld bead parameters, that is minimization of penetration and maximization of reinforcement and weld bead width , are made with a view to economize the input process parameters to achieve the desirable welding joint.

Keywords: PTA welding; Overlay; Stainless steel 316L; Colmonoy; Penetration; Reinforcement; Regression analysis; Mathematical model; Optimization I. Introduction Weld deposition of hard facing alloys is commonly employed to e n h a n c e t h e t r i b o l o g i c a l l i f e o f Engineering c o m p o n e n t s subjected to hostile environments. There clamation of worn-out metal parts is demanded worldwide and for this demand PTA hard facing of hard, wear resistant thin surface layer of metals and alloys on suitable substrates is one of the proven surfacing techniques(7).In the recent years, PTA Surfacing is extensive used in applications such as valve industries, Hydraulic machineries, Mining industries, Earthmoving equipment, Chemical, Nuclear and Thermal power plants etc.PTA process can be considered as an advanced Gas Tungsten Arc welding process more widely used for overlay applications. The metal and alloy powder is carried from the powder feeder to the central electrode holder in the arc-gas stream. From the electrode holder the powder is directed to the constricted arc zone, where it is melted and fusion bonded to the base metal. Thus, smooth, thin deposits of overlays can be made through this way of precise control of feed stock by PTA welding process. Colmonoy5, a Nickel based alloy (Ni-Cr-B-Si-C) provides excellent resistance to abrasive and adhesive wear with resistance to corrosion and high temperature oxidation. It is widely applied in Thermal power plants, Chemical industries, Nuclear reactors, food processing industries etc. In nuclear reactors, use of Co based satellite alloys lead to induced activity which will harm the personnel involved in the maintenance o f r e a c t o r c o m p o n e n t s . Colmonoy5 is a good alternative to the Co based alloys used (9, 15) in nuclear applications, fabricated wearers instant bushes are made of har d facin g allo ys fo r hi gh te mp eratur e ap p licatio ns . They report that there is a growing tendency to replace Co based alloys by Nickel based alloys, due to the high cost and scarcity of cobalt based alloys. The problem of cracking susceptibility of nickel based Colmonoy alloy hard faced deposits can be controlled by using preheating and slow cooling during deposition. Compared to other welding processes PTA surfacing requires less quantity of material to be deposited with improved mechanical and metallurgical properties.

Figure 1: Weld bead geometry The shape of the weld bead geometry is affected by the values of PTA process parameters used in deposition. These process parameters should be well established and categorized to enable automation and robotisation of PTA surfacing. Therefore it is imperative to develop mathematical models to predict the bead geometry and study the direct effects of various PTA process parameters on the weld bead shapes. The selection of w e l d i n g procedure must b e mo r e s p e c i f i c t o e n s u r e t h a t adequate bead quality is obtained(8).Further a complete control over the process parameters is essential to www.ijmer.com

1330 | Page

www.ijmer.com

International Journal of Modern Engineering Research (IJMER) Vol.3, Issue.3, May-June. 2013 pp-1330-1335 ISSN: 2249-6645

produce quality welds with required bead geometry based on which the integrity of the weldment is known. It has been reported by researchers that in PTA surfacing, process quality can be represented by bead shape (11). Thus the weld pool geometry plays an important role in deter mining the mechanical and corrosion properties of the weld. Therefore, process parameters for obtaining optimal weldpool geometry. It is reported that five level factorial techniques can be employed for developing models to predict weld bead geometry(1,5,6,12,13).In this work, automatic PTA hard facing is carried out for depositing Colmonoy5 over Stainless steel 316L plates of size 150mmx90mmx30mm.The experiments are based on the central composite rotatable design matrix. Regression analysis was used to develop the model. Also, the main objective of this study is to optimize the weld bead parameters that is achieving minimum penetration, maximum reinforcement and maximum bead width which gives best weld joint and determining the corresponding process parameters. Penetration means the depth into substrate through which the filler metal penetrates. Reinforcement means height of filler metal on substrate. Weld width means the width of filler metal on substrate.

II. The Work To Be Carried Out Was Planned In The Following Order 1. 2. 3. 4. 5. 6. 7. 8. 9. 10.

Identification of important process parameters Finding the upper and lower limits with different levels of the identified process parameters Development of Design matrix. Conducting experiments as per the design matrix Recording the responses Calculation of regression coefficients and development of mathematical model Development of final mathematical model Presenting the relation of process variables on bead geometry in graphical form. Results and discussions. O p t i m i z a t i o n o f we l d b e a d p a r a me t e r .

Identification of Process parameters- The independently controllable process parameters identified based on their significant effect on weld bead geometry to carry out the experimental work are welding current(A),Oscillation width(O),Travel speed(S),Preheat temperature(T) and Powder feed rate(F) g a s fl o w r a t e a n d T o r c h s t a n d o f f distance. W e l d i n g c u r r e n t p r o d u c e h e a t f o r f u s i o n , Pre heat temperature and oscillation width (17) which may affect crack formation during hard facing, have to be properly c o n t r o l l e d . M i n i m u m t o r c h t r a v e l s p e e d g i v e s b e t t e r d e p o s i t i o n o f f i l l e r m a t e r i a l o n we l d i n g j o i n t s . In deposition of material the most effective process parameters are Welding current, Oscillation width, Travel speed, Preheat temperature and Powder feed rate, thus these process parameters are selected in the experiment and the G a s fl o w r a t e a n d T o rc h s t a n d o f f distance are kept at constant levels. Limits and Levels of Process Parameters- It has been observed from different experiments that best deposition of nickel on steel plate occurs when the process parameters vary between the levels given in table 1.The working ranges of all selected parameters are fixed by conducting trial runs. This are carried out by varying one parameter while keeping the rest of them at constant values. The working range of each process parameter is decided upon by inspecting the bead for a smooth appearance without any visible defects. The upper limit of a factor is coded as +2, in between levels is -1, 0,1and the lower limit is coded as-2. The chosen levels of the process parameters and notations are given in Table1. Table 1: Levels of Process Variable

Development of design matrix- The design matrix is developed according to the combinations normally taken in Genetic Algorithm process for five process parameters. The design matrix chosen to conduct the experiment is a central composite rotatable design. It consists of 32sets of coded conditions and comprising a half replication of 24=16 factorial design with 6centre points and 10 star points .All the welding parameters at the middle level (0) constitute centre points whereas the combination of each welding parameter at its lower value (-2) or higher value (2) with the other four parameters at the middle levels constitute the star points (2, 10, 14). Thus the 32 experimental runs allowed the estimation of linear, quadratic and two-way interactive effects of the process parameters on the weld bead geometry. www.ijmer.com

1331 | Page

www.ijmer.com

International Journal of Modern Engineering Research (IJMER) Vol.3, Issue.3, May-June. 2013 pp-1330-1335 ISSN: 2249-6645

Experimental setup and procedure- The experiments are conducted by using a PTA welding machine, fabricated by National Automation Calcutta. Experiments are conducted by company and corresponding data are taken from their experiments. The PTA system has six modules namely traverse carriage unit, oscillator unit, powder feed unit, water-cooling unit, turntable unit and torch unit. All the units are supporting the effective functioning of the total PTA system. The experiments are conducted according to the design matrix at random to avoid systematic errors creeping into the system. Colmonoy 5 is deposited over stainless steel 316L plates 15cm x 9 cm.x3cm..Torch standoff distance, oscillating frequency, plasma/central gas flow rate, shielding gas flow rate and powder/carrier gas flow rate are kept constant respectively at10mm, 72cycles per minute, 3.5lpm, 12 lpm and 1.5 lpm while hard facing. Experimental observation- The hard faced plates were cross sectioned at their midpoints to get the test samples. Those samples are prepared by the usual metallographic polishing methods and etched with aquaregia solution for carrying out weld bead geometry measurements. The profiles of the weld beads and the bead dimensions i.e. Penetration (P), reinforcement (R) and weld width (W) are measured. The observed values of P, R and W are given in Table: 2. Table 2: Design Matrix and Observed Values Of Weld Bead Dimensions

III. Development Of Mathematical Models The response function representing any of the weld bead dimensions like penetration ,reinforcement etc, can be expressed as Y=f(A,O,S,T,F),Where Y is the response or yield .The second order polynomial (regression equation) use to represent the response surface for k factors are given by: Y= b0+

đ?‘˜ đ?‘–=1 đ?‘?đ?‘– đ?‘Ľđ?‘– +

đ?‘˜ 2 đ?‘–=1 đ?‘?đ?‘–đ?‘– đ?‘Ľđ?‘– đ?‘–â‰ đ?‘—

+

đ?‘˜ đ?‘–đ?‘— =1 đ?‘?đ?‘–đ?‘—

đ?‘Ľđ?‘– đ?‘Ľđ?‘— â€Śâ€Śâ€Śâ€Śâ€Śâ€Śâ€Ś..â€Śâ€Ś (1)

The selected polynomial for five factors can be expressed: Y=bo+b1A+b2O+b3S+b4T+b5F+b11A2+b22O2+b33S2+b44T2+b55F2+b12AO+b13AS+b14AT+b15AF+b23OS+ b24OT+b25OF +b34ST+b35SF +b45TF â€Ś(2) Where bo is free term of the regression equation, the coefficients b1, b2, b3, b4, and b5 are linear terms, the coefficients b11, b22, b33, b44, and b55 are quadratic terms, and the coefficients b12, b13, b14, b15, b23, b24, b25, b34, b35 and b45 are interaction terms. Development of final mathematical model: The co-efficient of the polynomials has been found by using MATLAB.Software. The final mathematical models determined by the regression analysis are as follows: P=0.95063+0.252A-0.038O-0.107S-0.063T-0.134F+0.027A2+0.0368O2-0.025S2+0.111T2-0.016F2+0.072AO0.028AS+0.159AT-0.027AF +0.110OS-0.091OT-0.064OF+0.122ST+0.092SF+0.023TF â€Ś. (3) R=3.514-0.003A-0.179O-0.074S+0.020T+0.048F-0.049A2-0.014O2-0.045S2-0.074T2-0.012F2+0.089AO0.026AS+0.036AT+0.051AF+0.053OS+0.043OT-0.059OF+0.043ST-0.0029SF-0.037TF â€Ś. â€Śâ€Śâ€Ś (4) W=18.96+0.856A+1.11O-0.346S-0.220T+0.093F+0.164A2+0.164O2+0.189S2+0.033T2+0.064F2+0.253AO0.303AS+0.284AT-0.088AF+0.212OS-0.080OT-0.171OF+0.105ST+0.1714SF-0.165TF â€Ś (5) www.ijmer.com

1332 | Page

www.ijmer.com

IV.

Result And Discussion

The developed mathematical models can be used to predict the dimensions of the weld bead. Based on these models, the effects of process parameters on bead dimensions are computed and plotted by varying one parameter and keeping others at middle value. It is also possible to substitute the values for bead dimensions and get the corresponding values of PTA process parameters in coded form. Discussion

Figure 2: Direct effect of process variables on penetration Direct effects of Process variables on Penetration Figure2 shows that Penetration (P) increases significantly when welding current increases. This is attributed to the fact that heat input to the base metal increases when current is increased. Penetration decreases as Oscillation width increases. This is due to spreading of heat resulting from more melting of base metal. Penetration decreases steadily with the increase of Travel speed as less amount of powder is deposited per unit length of bead. Penetration decreases to a lower value when pre heat temperature increases but afterwards penetration increases with further increase of preheat temperature. This may be for the reasons that at lower preheat temperature the heat received from plasma arc will not spread in the stainless steel substrate due to lower thermal conductivity resulting in cushioning of arc. Penetration decreases with increase of Powder feed rate.

Figure 3: Direct effect of process variables on reinforcement Direct effect of Process variables on Reinforcement It is evident from Fig 3 that Reinforcement (R) increases initially and then decreases with increase of welding current. Reinforcement decreases with increase in oscillation width. This could possibly due to the fact that the deposited metal gets distributed along the width resulting in decreasing in reinforcement. Reinforcement decreases steadily from highest value with the increase of travel speed. This is due to reduce amount of powder deposit per unit length of bead. Reinforcement increases with increase of preheat temperature to its peak value then decreases with further increase of preheat temperature. Reinforcement increases steadily with increase of powder feed rate as more powder is deposited per unit length of weld bead.

www.ijmer.com

1333 | Page

www.ijmer.com

Figure 4: Direct effect of process variables on weld with Direct effects of Process variables on Weld width Figure 4 show that Weld width increases with increase of welding current .This is due to spreading of heat resulting of melting of more metal. Weld width increases steadily with increase in oscillation width due to decrease of Penetration. Weld bead decreases with increase of torch travel speed .This may be for reduced heat input per unit length of weld bead when travel speed is increased. Weld bead width reduces as the Preheat temperature increases. Weld width decreases initially but increases with increase of powder feed rate. A better weld should have bead parameters as follows 1. Penetration should be minimum 2. Reinforcement should be maximum 3. Weld width should be maximum The bead parameters are found independently considering their equations obtain from mathematical modeling as objective function. The best weld bead parameters are found by analyzing the graph between weld bead parameters and process parameters .The best weld bead parameters and the corresponding process parameters are as follow

A(amps) 120 (-2)

A( amps) 140 (0)

A ( amps ) 160 (2)

a) Minimization of depth of penetrationO(mm) S(mm/min ) T(◦c) 18 (2) 107(2) 300(0) Predicted minimum penetration = 0.463mm

F(gm./min) 44(2)

b) Maximization of height of reinforcementO( mm) S(mm/min) T( ◦c) 10 (-2) 79 (-2) 300(0) Predicted maximum reinforcement =4.29mm

F(gm/min) 44(2)

c) Maximization of weld widthO(mm) S(mm/min) T(◦c) 18 (2) 79 (-2) 250(-2) Predicted maximum weld width =26.58mm

F (gm/min) 44 (2)

Hence the best of bead parameters for different sets of process variable is as follows 1. Penetration=0.463mm 2. Reinforcement = 4.29mm 3. Weld width = 26.58mm

V.

Optimization

It is very difficult for an operator to perform the welding process to get best bead parameters using different sets of process variable. Hence it is necessary to find a single set of process variable which will provide the optimal bead parameters and are very close to the best bead parameters find with different sets of process variable. Here optimization of the bead parameters is done by considering the three sets of process variable obtained for best bead parameters as mentioned above. All possible combinations of process variables are carried by using MATLAB software and the corresponding bead parameters are recorded, neglecting negative ones. It can be seen that there are 24 sets of valid process variables giving as many sets of bead parameters. It is found from results that optimum set of bead parameter is as follows www.ijmer.com

1334 | Page

www.ijmer.com

The process variables and corresponding optimum bead parameters are given below. Table 3: Optimized values of bead parameters and corresponding process variables A (amp) O(mm) S(mm/min) F (gm./min) P(mm) R(mm) T(℃) 160(2) 18(2) 79(-2) 300(0) 44(2) 0.640 3.1358

W(mm) 25.768

Condition for better welding joint 1. Higher amperage produces higher welding temperature which interns produces better fusion of metal. Better fusion produces better weld 2. More oscillation width produces more weld width. 3. Less travel speed of torch produces better reinforcement. 4. Medium pre heat temperature reduces the chance of cracking. 5. More powder feed rate produces more reinforcement. According to the theory the best combination of process variables for optimum bead parameters should be as follows Table 4: Combination of process variables for optimum bead parameters A(amps) O(mm) S(mm/min) T ( ◦c) F(gm/min) 160(2) 18(2) 79(-2) 300(0) 44(2) Accordingly the predicted bead parameters for this set are as follows Penetration is 0.640 mm, Reinforcement is 3.1358mm Weld bead is25.768 mm This is exactly the same set of bead parameters obtain by the optimization process. Hence it can be said that the optimization process is justifying the theory. Comparison of the bead parameter received from different sets and single set of process variable. Result obtain for best bead parameters for different sets of Result obtain for optimum bead parameters using single process variables set of process variables Penetration 0.463mm

Reinforcement 4.29mm

Weld width 26.58mm

Penetration 0.640mm

Reinforcement 3.135mm

Weld width 25.768mm

Bibliography [1] [2] [3] [4] [5] [6] [7] [8] [9] [10] [11] [12] [13] [14] [15] [16] [17]

T.T.Allen, R.W.Richardson, D.P.Tagliable, G.P. Maul, Statistical processdesignforrobotic GMAweldingofsheet metal, Welding Journal 81/5(2002)69-172. W.G. Cochran, G.M. Cox, Experimental Designs, John Willy & sons Singapore 1957 C.R. Das, S.K. Albert, A.K., Bhaduri, G. Kempulraj, A novel procedure for fabrication of wearresistantbushes for high temperature application, Journal of Materials Processing Technology141(2003)60-66. H. Eschnauer, Hard material powders and hard alloy powders for plasmas face coating, Thin Solid Films73 1980 pp 1-17. B. Howard, Surfacing for wear resistance, Stephen Helbaet al. (eds.), Modern Welding Technology, Prentice HallInc., New Jersey, 2022pp 721-726 I.S.Kim, J.S.Son, Y.J.Jeung, Control and Optimisation of bead widthformulti-passwelding inroboticarcwelding processes, Australian Welding Journal 46 (2001)43-46 R.Kaul,P.Ganesh,S.K.Albert,A.Jaishwal,N.P.Lalla,A. Gupta C.P.Pal ,A.K.NathLasercladdingof austenitic stainless steel with nickel base hard facing alloy, Surface Engineering19 (2003)pp269-273. K.Marimuthu, N.Murugan Prediction and optimization of weld bead geometry of Plasma transferred arc hard faced valve seat rings, Surface Engineering19/2(2003) 143-149. J.C.Mc.Glone, Weldbeadgeometryprediction –areview, Metal Construction14 (1982)378-384. D.C. Montgomery, Designand analysis of experiments, John Wiley&SonsInc., New York, 2001. P.K. Palani, N. Murugan, O p t i m i z a t i o n ofweld bead geometry of stainless steel cladding by flux Cored arc welding using Excel Solver, IWS Journal 2 (2005)15-19. A. Scotti, L.Alves, Albuquerque Rosa, Influence of oscillation parameter soncrack for mationin automaticFe-B hard facing, Journal of Materials Processing Technology 65 (1997)272-280. K.Y.Benyounis and A.G.OlbiOptimization of PTA welding process using Statistical and Numerical approach. (2005) Marimuthu and Murugan Effects of Plasma Transferred Arc Welding parameters on welding bead geometry, in computational materials science and surface engineering vol. 8 pp 51-88 (2006) Keung –Hueng Teseng et.al.Optimization of PTAW parameters. Journal of manufacturing science and production vol.10 pp 155-188 (2008) Siva, K.Murugan and Raghupathy Modelling, analysis and optimization of weld bead parameters of PTAW, computional materials science and surface engineering vol.1 pp 174-182 (2009) R .Logesh, K.Siva, N.Murugan, Optimization of weld bead geometry in PTAW hard faced on austenitic stainless steel plate using genetic algorithm. International journal of advanced manufacturing technology vol.41 pp 24-30

www.ijmer.com

1335 | Page

Advertisement